 Download Download Presentation Chapter 6. Mechanical Behavior

# Chapter 6. Mechanical Behavior

Download Presentation ## Chapter 6. Mechanical Behavior

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -
##### Presentation Transcript

1. Chapter 6. Mechanical Behavior • Stress versus Strain • Elastic Deformation • Plastic Deformation • Hardness • Creep and Stress Relaxation • Viscoelastic Deformation

2. Stress versus Strain • Mechanical Properties • Deal directly with behavior of materials under applied forces. • Properties are described by applied stress and resulting strain, or applied strain and resulting stress. • Example: 100 lb force applies to end of a rod results in a stress applied to the end of the rod causing it to stretch or elongate, which is measured as strain. • Strength: ability of material to resist application of load without rupture. • Ultimate strength- maximum force per cross section area. • Yield strength- force at yield point per cross section area. • Other strengths include rupture strength, proportional strength, etc. • Stiffness: resistance of material to deform under load while in elastic state. • Stiffness is usually measured by the Modulus of Elasticity (Stress/strain) • Steel is stiff (tough to bend). Some beds are stiff, some are soft (compliant)

3. Testing Procedures • Mechanical Testing • Properties that deal with elastic or inelastic behavior of a material under load • Primary measurements involved are load applied and effects of load application • Two classification of tests; method of loading and the condition of the specimen during the test • Primary types of tests • Tensile • Compression • Shear • Torsion • Flexure

4. Mechanical Test Considerations shear • Principle factors are in three main areas • manner in which the load is applied • condition of material specimen at time of test • surrounding conditions (environment) during testing • Tests classification- load application • kind of stress induced. Single load or Multiple loads • rate at which stress is developed: static versus dynamic • number of cycles of load application: single versus fatigue • Primary types of loading compression tension torsion flexure

5. Standardized Testing Conditions • Moisture • 100F, 100% R.H. • 1 Day, 7 Days, 14 Days • Temperature • Room Temperature: Most common • Elevated Temperature: Rocket engines • Low Temperature: Automotive impact • Salt spray for corrosion • Rocker Arms on cars subject to immersion in NaCl solution for 1 Day and 7 Days at Room Temperature and 140 F. • Acid or Caustic environments • Tensile tests on samples after immersion in acid/alkaline baths.

6. Stress • Stress: Intensity of the internally distributed forces or component of forces that resist a change in the form of a body. • Tension, Compression, Shear, Torsion, Flexure • Stress calculated by force per unit area. Applied force divided by the cross sectional area of the specimen. • Stress units • Pascals = Pa = Newtons/m2 • Pounds per square inch = Psi Note: 1MPa = 1 x106 Pa = 145 psi • Example • Wire 12 in long is tied vertically. The wire has a diameter of 0.100 in and supports 100 lbs. What is the stress that is developed? • Stress = F/A = F/r2 = 100/(3.1415927 * 0.052 )= 12,739 psi = 87.86 MPa

7. Stress 0.1 in 1 in 10in • Example • Tensile Bar is 10in x 1in x 0.1in is mounted vertically in test machine. The bar supports 100 lbs. What is the stress that is developed? What is the Load? • Stress = F/A = F/(width*thickness)= 100lbs/(1in*.1in )= 1,000 psi = 1000 psi/145psi = 6.897 Mpa • Load = 100 lbs • Block is 10 cm x 1 cm x 5 cm is mounted on its side in a test machine. The block is pulled with 100 N on both sides. What is the stress that is developed? What is the Load? • Stress = F/A = F/(width*thickness)= 100N/(.01m * .10m )= 100,000 N/m2 = 100,000 Pa = 0.1 MPa= 0.1 MPa *145psi/MPa = 14.5 psi • Load = 100 N 100 lbs 1 cm 5cm 10cm

8. Strain lF l0 • Strain: Physical change in the dimensions of a specimen that results from applying a load to the test specimen. • Strain calculated by the ratio of the change in length and the original length. (Deformation) • Strain units (Dimensionless) • When units are given they usually are in/in or mm/mm. (Change in dimension divided by original length) • % Elongation = strain x 100%

9. Strain 0.1 in 1 in 10in • Example • Tensile Bar is 10in x 1in x 0.1in is mounted vertically in test machine. The bar supports 100 lbs. What is the strain that is developed if the bar grows to 10.2in? What is % Elongation? • Strain = (lf - l0)/l0 = (10.2 -10)/(10)= 0.02 in/in • Percent Elongation = 0.02 * 100 = 2% • Block is 10 cm x 1 cm x 5 cm is mounted on its side in a test machine. The block is pulled with 1000 kN on bone side. If the material elongation at yield is 1.5%, how far will it grow at yield? • Strain = Percent Elongation /100 = 1.5%/100 = 0.015 cm /cm • Strain = (lf - l0)/l0 = (lf -5)/(5)= 0.015 cm/cm • Growth = 5 * 0.015 = 0.075 cm • Final Length = 5.075 cm 100 lbs 1 cm 5cm 10cm

10. Strain • Permanent set is a change in form of a specimen once the stress ends. • Axial strain is the strain that occurs in the same direction as the applied stress. • Lateral strain is the strain that occurs perpendicular to the direction of the applied stress. • Poisson’s ratio is ratio of lateral strain to axial strain. Poisson’s ratio = lateral strain axial strain • Example • Calculate the Poisson’s ratio of a material with lateral strain of 0.002 and an axial strain of 0.006 • Poisson’s ratio = 0.002/0.006 = 0.333 Lateral Strain Axial Strain • Note: For most materials, Poisson’s ratio is between 0.25 and 0.5 • Metals: 0.29 (304 SS) to 0.3 (1040 steel) to 0.35 (Mg) • Ceramics and Glasses: 0.19 (TiC) to 0.26 (BeO) to 0.31 (Cordierite) • Plastics: 0.35 (Acetals) to 0.41 (Nylons)

11. Stress-Strain Diagrams • Equipment • Strainometers: measures dimensional changes that occur during testing • extensometers, deflectometers, and compressometers measure changes in linear dimensions. • load cells measure load • data is recorded at several readings and the results averaged, e.g., 10 samples per second during the test.

12. Stress-Strain Diagrams Linear (Hookean) Stress Non-Linear (non-Hookean) Strain • Stress-strain diagrams is a plot of stress with the corresponding strain produced. • Stress is the y-axis • Strain is the x-axis

13. Stiffness • Stiffness is a measure of the materials ability to resist deformation under load as measured in stress. • Stiffness is measures as the slope of the stress-strain curve • Hookean solid: (like a spring) linear slope • steel • aluminum • iron • copper • All solids (Hookean and viscoelastic) • metals • plastics • composites • ceramics

14. Modulus • Modulus of Elasticity (E) or Young’s Modulus is the ratio of stress to corresponding strain (within specified limits). • A measure of stiffness • Stainless Steel E= 28.5 million psi (196.5 GPa) • Aluminum E= 10 million psi • Brass E= 16 million psi • Copper E= 16 million psi • Molybdenum E= 50 million psi • Nickel E= 30 million psi • Titanium E= 15.5 million psi • Tungsten E= 59 million psi • Carbon fiber E= 40 million psi • Glass E= 10.4 million psi • Composites E= 1 to 3 million psi • Plastics E= 0.2 to 0.7 million psi

15. Modulus Types Stress Strain • Modulus: Slope of the stress-strain curve • Initial Modulus: slope of the curve drawn at the origin. • Tangent Modulus: slope of the curve drawn at the tangent of the curve at some point. • Secant Modulus: Ratio of stress to strain at any point on curve in a stress-strain diagram. It is the slope of a line from the origin to any point on a stress-strain curve. Initial Modulus Tangent Modulus Secant Modulus

16. Compression Testing l0 lF • Principles • Compression results from forces that push toward each other. • Specimens are short and large diameter. • Circular cross section is recommended. • Length to diameter ratio is important consideration • Universal test machine (UTM) • Size and load of compression machine are specially built. • Load and compression amount are measured. • Stress • Force per unit area. Applied force divided by the cross sectional area of the specimen. • Strain calculated by the ratio of the change in length and the original length. (Deformation)

17. Expected Results Stress Strain • Similar Stress-strain curve as tensile testing

18. Shear Testing • Principles • Direct shear occurs when parallel forces are applied in the opposite direction. • Single shear occurs on a single plane. • Double shear occurs on two planes simultaneously.

19. Shear Testing • Principles • Torsional shearing forces occur when the forces applied lie in parallel but opposite directions. Twisting motion. • Torsional forces developed in a material are the result of an applied torque. • Torque is Forces x distance.. • Universal test machine (UTM) • Special fixtures are needed to hold the specimen. • One end of the specimen is placed in a fixture that applies torsional load and the other end is connected to a tropometer, which measures the detrusion (load and deflection or twist)

20. Expected Results Stress Strain • Similar Stress-strain curve as tensile testing

21. Bend of Flexure Testing • Principles • Bending forces occur when load is applied to a beam or rod that involves compression forces on one side of a beam and tensile forces on the other side. • Deflection of a beam is the displacement of a point on a neutral surface of a beam from its original position under action of applied loads. • Flexure is the bending of a material specimen under load. • Strength that material exhibits is a function of the flexural modulus of the material and the cross-sectional geometry. • Example, rectangular beam of 1” x 4” (W) will exhibit higher flexural strength than a 2” by 2” square beam of the same material modulus. • Properties are the same as in tensile testing. • Strength, deflection, modulus, ultimate strength, etc. • Specimen is loaded in a 3-point bending test • bottom goes in tension and the top goes in compression. • Failure analysis can provide information as the type of failure, • either tension or compression failure, • buckle prior to failure, • condition of fracture, e.e., rough, jagged, or smooth.

22. Equipment • Universal test machine (UTM) • Special fixtures are needed to hold the specimen. • Precautions • Specimen length should be 6 to 12 times the width to avoid shear failure or buckling. • Areas of contact with the material under test should be such that unduly high stress concentrations are avoided. • Longitudinal adjustments are necessary for the supports. • Lateral rotational adjustments should be provided to prevent torsional stresses. • The parts should be arranged to be stable under load.

23. Expected Results Stress Strain • Similar Stress-strain curve as tensile testing

24. Impact Testing • Principles • Materials exhibit different properties depending on the rate at which a load is applied and the resulting strain that occurs. • If a load is applied over a long period of time (static test)the material can withstand greater loads than if the test is applied rapidly (dynamic). • Properties of materials are stain dependent. • Standardized tests are used to determine the amount of energy required to break a material in impact tests. • Outcome of impact tests is to determine the amount of energy needed to break a sample.

25. Impact Testing • Principles • Energy absorbed in several ways • Elastic deformation of the members or parts of a system. • Plastic deformation. • Hysteresis effects. • Frictional action • effects of inertia on moving parts. • Energy is defined as the ability to do work. E =W = F*D • Work is Force times distance moved. • Energy of a dropped object hitting a specimen is • E = w*h Energy is weight times height dropped. • E = m*g*h (metric) Energy is mass times gravity acceleration times height.

26. Equipment • Impact Testing Equipment • Izod and Charpy are the most common tests. • Both employ a swinging pendulum and conducted on small notched specimens. The notch concentrated the load at a point causing failure. Other wise without the notch the specimen will plastically deform throughout. • They are different in the design of the test specimen and the velocity at which the pendulum strikes the specimen. • Charpy: the specimen is supported as a single beam and held horizontally. Impacted at the back face of the specimen. • Izod: the specimen is supported as a cantilever and help vertically. Impacted at front face of the specimen. • Figure 19-1

27. Impact Test • In standard testing, such as tensile and flexural testing, the material absorbs energy slowly. • In real life, materials often absorb applied forces very quickly: falling objects, blows, collisions, drops, etc. • A product is more likely to fail when it is subjected to an impact blow, in comparison to the same force being applied more slowly. • The purpose of impact testing is to simulate these conditions.

28. Impact Test • Impact testing is testing an object's ability to resist high-rate loading. • An impact test is a test for determining the energy absorbed in fracturing a test piece at high velocity. • Most of us think of it as one object striking another object at a relatively high speed. • Impact resistance is one of the most important properties for a part designer to consider, and without question the most difficult to quantify. • The impact resistance of a part is, in many applications, a critical measure of service life. More importantly these days, it involves the perplexing problem of product safety and liability. • One must determine: • 1.the impact energies the part can be expected to see in its lifetime, 2.the type of impact that will deliver that energy, and then 3.select a material that will resist such assaults over the projected life span. • Molded-in stresses, polymer orientation, weak spots (e.g. weld lines or gate areas), and part geometry will affect impact performance. • Impact properties also change when additives, e.g. coloring agents, are added to plastics.

29. Impact Test • Most real world impacts are biaxial rather than unidirectional. • Plastics, being anisotropic, cooperate by divulging the easiest route to failure. • Complicated choice of failure modes: Ductile or brittle. • Brittle materials take little energy to start a crack, little more to propagate it to a shattering climax. • Highly ductile materials fail by puncture in drop weight testing and require a high energy load to initiate and propagate the crack. • Many materials are capable of either ductile or brittle failure, depending upon the type of test and rate and temperature conditions. • They possess a ductile/brittle transition that actually shifts according to these variables. • For example, some plastic food containers are fine when dropped onto the floor at room temperature but a frozen one can crack when dropped.

30. Expected Results • Charpy Test • Capacity of 220 ft-lb for metals and 4 ft-lbs for plastics • Pendulum swings at 17.5 ft/sec. • Specimen dimensions are 10 x 10 x 55 mm, notched on one side. • Procedure • Pendulum is set to angle, , and swings through specimen and reaches the final angel, . If no energy given then  = . • Energy is

31. Expected Results • Izod Test • Capacity of 120 ft-lb for metals and 4 ft-lbs for plastics • Impacted at the front face of the specimen. • Specimen dimensions are 10 x 10 x 75 mm, notched on one side. • Procedure • Pendulum is set to angle, , and swings through specimen and reaches the final angel, . If no energy given then  = . • Energy is

32. Fundamentals of Hardness • Hardness is thought of as the resistance to penetration by an object or the solidity or firmness of an object • Resistance to permanent indentation under static or dynamic loads • Energy absorption under impact loads (rebound hardness) • Resistance toe scratching (scratch hardness) • Resistance to abrasion (abrasion hardness) • Resistance to cutting or drilling (machinability) • Principles of hardness (resistance to indentation) • indenter: ball or plain or truncated cone or pyramid made of hard steel or diamond • Load measured that yields a given depth • Indentation measured that comes from a specified load • Rebound height measured in rebound test after a dynamic load is dropped onto a surface

33. Hardness Mechanical Tests • Brinell Test Method • One of the oldest tests • Static test that involves pressing a hardened steel ball (10mm) into a test specimen while under a load of • 3000 kg load for hard metals, • 1500 kg load for intermediate hardness metals • 500 kg load for soft materials • Various types of Brinell • Method of load application:oil pressure, gear-driven screw, or weights with a lever • Method of operation: hand or electric power • Method of measuring load: piston with weights, bourdon gage, dynamoeter, or weights with a lever • Size of machine: stationary (large) or portable (hand-held)

34. Brinell Test Conditions • Brinell Test Method (continued) • Method • Specimen is placed on the anvil and raised to contact the ball • Load is applied by forcing the main piston down and presses the ball into the specimen • A Bourbon gage is used to indicate the applied load • When the desired load is applied, the balance weight on top of the machine is lifted to prevent an overload on the ball • The diameter of the ball indentation is measured with a micrometer microscope, which has a transparent engraved scale in the field of view

35. Brinell Test Example • Brinell Test Method (continued) • Units: pressure per unit area • Brinell Hardness Number (BHN) = applied load divided by area of the surface indenter Where: BHN = Brinell Hardness Number L = applied load (kg) D = diameter of the ball (10 mm) d = diameter of indentation (in mm) • Example: What is the Brinell hardness for a specimen with an indentation of 5 mm is produced with a 3000 kg applied load. • Ans:

36. Brinell Test Method (continued) • Range of Brinell Numbers • 90 to 360 values with higher number indicating higher hardness • The deeper the penetration the higher the number • Brinell numbers greater than 650 should not be trusted because the diameter of the indentation is too small to be measured accurately and the ball penetrator may flatten out. • Rules of thumb • 3000 kg load should be used for a BHN of 150 and above • 1500 kg load should be used for a BHN between 75 and 300 • 500 kg load should be used for a BHN less than 100 • The material’s thickness should not be less than 10 times the depth of the indentation

37. Advantages & Disadvantages of the Brinell Hardness Test • Advantages • Well known throughout industry with well accepted results • Tests are run quickly (within 2 minutes) • Test inexpensive to run once the machine is purchased • Insensitive to imperfections (hard spot or crater) in the material • Limitations • Not well adapted for very hard materials, wherein the ball deforms excessively • Not well adapted for thin pieces • Not well adapted for case-hardened materials • Heavy and more expensive than other tests (\$5,000)

38. Rockwell Test • Hardness is a function of the degree of indentation of the test piece by action of an indenter under a given static load (similar to the Brinell test) • Rockwell test has a choice of 3 different loads and three different indenters • The loads are smaller and the indentation is shallower than the Brinell test • Rockwell test is applicable to testing materials beyond the scope of the Brinell test • Rockwell test is faster because it gives readings that do not require calculations and whose values can be compared to tables of results (ASTM E 18)

39. Rockwell Test Description • Specially designed machine that applies load through a system of weights and levers • Indenter can be 1/16 in hardened steel ball, 1/8 in steel ball, or 120° diamond cone with a somewhat rounded point (brale) • Hardness number is an arbitrary value that is inversely related to the depth of indentation • Scale used is a function of load applied and the indenter • Rockwell B- 1/16in ball with a 100 kg load • Rockwell C- Brale is used with the 150 kg load • Operation • Minor load is applied (10 kg) to set the indenter in material • Dial is set and the major load applied (60 to 100 kg) • Hardness reading is measured • Rockwell hardness includes the value and the scale letter

40. Rockwell Values • B Scale: Materials of medium hardness (0 to 100HRB) Most Common • C Scale: Materials of harder materials (> 100HRB) Most Common • Rockwell scales divided into 100 divisions with each division (point of hardness) equal to 0.002mm in indentation. Thus difference between a HRB51 and HRB54 is 3 x 0.002 mm - 0.006 mm indentation • The higher the number the harder the number

41. Rockwell and Brinell Conversion • For a Rockwell C values between -20 and 40, the Brinell hardness is calculated by • For HRC values greater than 40, use • For HRB values between 35 and 100 use

42. Rockwell and Brinell Conversion • For a Rockwell C values, HRC, values greater than 40, • Example, • Convert the Rockwell hardness number HRc 60 to BHN

43. Form of Polymers Melt Temp Tm Rubbery Increasing Temp Tg Glassy Polymer Form • Thermoplastic Material: A material that is solid, that possesses significant elasticity at room temperature and turns into a viscous liquid-like material at some higher temperature. The process is reversible • Polymer Form as a function of temperature • Glassy: Solid-like form, rigid, and hard • Rubbery: Soft solid form, flexible, and elastic • Melt: Liquid-like form, fluid, elastic

44. Glass Transition Temperature, Tg • Glass Transition Temperature, Tg: The temperature by which: • Below the temperature the material is in animmobile(rigid) configuration • Above the temperature the material is in a mobile (flexible) configuration • Transition is called “Glass Transition” because the properties below it are similar to ordinary glass. • Transition range is not one temperature but a range over a relatively narrow range (10 degrees). Tg is not precisely measured, but is a very important characteristic. • Tg applies to all polymers (amorphous, crystalline, rubbers, thermosets, fibers, etc.)

45. Glass Transition Temperature, Tg Amorphous Modulus (Pa) or (psi) Crystalline Tg Tg Tg -50C 50C 100C 150C 200C 250C -50C 50C 100C 150C 200C 250C Temperature Temperature • Glass Transition Temperature, Tg: Defined as • the temperature wherein a significant the loss of modulus (or stiffness) occurs • the temperature at which significant loss of volume occurs Vol.

46. Crystalline Polymers: Tm • Tm: Melting Temperature • T > Tm,The order of the molecules is random (amorphous) • Tm >T>Tg,Crystallization begins at various nuclei and the order of the molecules is a mixture of crystals and random polymers (amorphous). Crystallization continues as T drops until maximum crystallinity is achieved. The amorphous regions are rubbery and don’t contribute to the stiffness. The crystalline regions are unaffected by temperature and are glassy and rigid. • T < Tg,The amorphous regions gain stiffness and become glassy Melt Tm Temp Rubbery Decreasing Temp Tg Glassy Polymer Form

47. Crystalline Polymers Tg -50C 50C 100C 150C 200C 250C Temperature • Tg: Affected by Crystallinity level • High Crystallinity Level = high Tg • Low Crystallinity Level = low Tg Modulus (Pa) or (psi) High Crystallinity Medium Crystallinity Low Crystallinity Tg

48. Temperature Effects on Specific Volume Amorphous Specific Volume Crystalline Tg Tg -50C 50C 100C 150C 200C 250C • T > Tm, The amorphous polymer’s volume decreases linearly with T. • Tm > T>Tg, As crystals form the volume drops since the crystals are significantly denser than the amorphous material. • T < Tg, the amorphous regions contracts linearly and causes a change in slope Temperature

49. Elastomers • Elastomers are rubber like polymers that are thermoset or thermoplastic • butyl rubber: natural rubber • thermoset: polyurethane, silicone • thermoplastic: thermoplastic urethanes (TPU), thermoplastic elastomers (TPE), thermoplastic olefins (TPO), thermoplastic rubbers (TPR) • Elastomers exhibit more elastic properties versus plastics which plastically deform and have a lower elastic limit. • Rubbers have the distinction of being stretched 200% and returned to original shape. Elastic limit is 200%

50. Rubbers • Rubbers have the distinction of being stretched 200% and returned to original shape. Elastic limit is 200% • Natural rubber (isoprene) is produced from gum resin of certain trees and plants that grow in southeast Asia, Ceylon, Liberia, and the Congo. • The sap is an emulsion containing 40% water & 60% rubber particles • Vulcanization occurs with the addition of sulfur (4%). • Sulfur produces cross-links to make the rubber stiffer and harder. • The cross-linkages reduce the slippage between chains and results in higher elasticity. • Some of the double covalent bonds between molecules are broken, allowing the sulfur atoms to form cross-links. • Soft rubber has 4% sulfur and is 10% cross-linked. • Hard rubber (ebonite) has 45% sulfur and is highly cross-linked.